Controlling aggregation-induced emission by supramolecular interactions and colloidal stability in ionic emitters for light-emitting electrochemical cells

Chromophores face applicability limitations due to their natural tendency to aggregate, with a subsequent deactivation of their emission features. Hence, there has been a fast development of aggregation induced emission (AIE) emitters, in which non-radiative motional deactivation is inhibited. However, a fine control of their colloidal properties governing the emitting performance is fundamental for their application in thin film optoelectronics. In addition, ion-based lighting devices, such as light emitting electrochemical cells (LECs), requires the design of ionic AIE emitters, whose structure allows (i) an easy ion polarizability to assist charge injection and (ii) a reversible electrochemical behavior. To date, these fundamental questions have not been addressed. Herein, the hydrophilic/hydrophobic balance of a family of cationic tetraphenyl ethene (TPE) derivatives is finely tuned by chemical design. The hydrophilic yet repulsive effect of pyridinium-based cationic moieties is balanced with hydrophobic variables (long alkyl chains or counterion chemistry), leading to (i) a control between monomeric/aggregate state ruling photoluminescence, (ii) redox behavior, and (iii) enhanced ion conductivity in thin films. This resulted in a LEC enhancement with the first ionic AIE emitters, reaching values of 0.19 lm W−1 at ca. 50 cd m−2. Overall, this design rule will be key to advance ionic active species for optoelectronics.


Introduction
][3][4] However, their use nds limitations due to the partial or complete emission quenching derived from aggregation, leading to the 'aggregation caused quenching' (ACQ).This is consequence of their usually large aromatic structures that lead to p-p stacking, and subsequently deactivates the photoexcited state(s) through non-radiative pathways. 5This phenomenon typically occurs at high concentrations, aqueous media given the high hydrophobicity of these derivatives, or the condensed/ solid state. 5,6Thus, aggregation limits their applicability as high payload imaging agents, phototherapeutic agents, or in lighting devices (e.g., OLEDs or solar cells), respectively.While chemical design of non-aggregating dyes, 7,8 or directed aggregation 9,10 has been pursued with success, a radically different approach has been explored to turn dye aggregation into a desirable feature.
Aggregation induced emission (AIE) is a photophysical phenomenon coined in 2001, in which aggregate formation enhances the light emitting process. 11,12AIE emitters (AIEgens) in their monomeric state suffer from emission quenching caused by intramolecular vibrations and rotations in e.g., organic solvents, leading to emission quenching.4][15] Consequently, AIEgens exhibit emitting properties in aggregate state.][18] Despite the plethora of AIEgen families, ionic AIE structures are understudied, likely given the a priori counterproductive properties: charged molecules will present enhanced aqueous solubility that, together with the coulombic repulsion, hinder self-assembly and, therefore, the AIE properties. 19For instance, ionic AIE probes have been used as protein labelling agents, with the AIE properties arising upon biomolecular recognition. 20However, a deep understanding of factors inuencing aggregation and monomeric states of ionic AIEgens in aqueous media and solid-state is crucial for controlling system forces and then, expanding applications (e.g.ultra-sensitive mechanochromic luminescent materials). 21In this context, ionic AIEgens present a unique potential for ionic-based optoelectronics, such as light-emitting electrochemical cells (LECs). 22hey are considered the simplest thin lm lighting device, in which the presence of ions in the active layer allows (i) an efficient charge injection from air stable electrodes, and (ii) a controlled electrochemical doping of the emitter forming a stable p-i-n junction, in which exciton radiative recombination occurs.Recently, Edman's group showed for the rst time that neutral AIE emitters with a rigid and emissive structure will be compatible with ionic electrolytes, realizing better devices than analogous emitters with typical ACQ. 23However, the use of ionic AIE emitters as well as the design principles to simultaneously merge desired photophysical, electrochemical, and ion transport for LECs remains unanswered.
5][26][27][28] They present a propeller-like structure formed by four phenyl groups moving freely in the monomeric state.The hydrophilic/ hydrophobic balance governing the AIE effect is nely tuned by the length of alkyl chain and the counterion: on one hand, the hydrophilicity is introduced by the positively charged pyridinium moieties that increase the solubility in aqueous media.On the other hand, the alkyl chain and the counterion nature modulate the hydrophobicity, and thus, overcoming electrostatic repulsions and promoting self-aggregation.We demonstrate the impact of the mentioned forces on the optical properties in organic solvent (monomeric) and aqueous media (monomeric or aggregate) at different concentrations in the series of halide TPPE-alkyl salts and hexauorophosphate (PF 6 − ) TPPE-alkyl salts.The length of the alkyl chains plays a key role on self-aggregation for TPPE-alkyl salts: C 12 chains are needed in order to turn on the AIE effect.PF 6 TPPE-alkyl salts, however, exhibit an enhanced AIE at lower concentrations and with shorter alkyl chains as well as a more reversible electrochemical behavior.Furthermore, we demonstrate the impact of the molecular structure in the electrochemical behavior and ion conductivity in thin lms.This series was further applied to LECs nicely showing that (i) the emission features of the lms enhance with the AIE behavior, (ii) the ion-assisted mechanism is fully operative and (iii) a linear trend to increase device gures of merit upon increasing the alkyl chain.This resulted in the rst LECs with ionic AIE emitters, exhibiting a yellow emission associated to ca.50 cd m −2 and 0.19 lm W −1 , which is in the range of small molecules LECs. 29
Photophysical properties of the halide TPPE-alkyl salts in solution.The synthesized family presents a ne-tuned hydrophilicity/hydrophobicity balance between the positively charged pyridinium moieties and the increasing chain length, respectively.On one hand, positive charges render aqueous solubility and coulombic repulsion render monomeric derivatives.On the other hand, long alkyl chains render aggregation in aqueous media, counterbalancing the electrostatic repulsion (Fig. 1a).The subtle interplay of forces has direct impact on the optical properties, in particular between the luminescence in organic solvent, i.e. methanol, and aqueous media (containing a 1% v/v fraction of the organic solvent).The rst renders the AIEgen in monomeric state, while the aqueous dispersion will either exhibit monomeric or aggregated (i.e., emitting) state, depending on the overall hydrophilicity/hydrophobicity balance.
First, the absorbance spectra of the halide TPPE-alkyl salts are recorded at different concentrations, both in organic and aqueous media (A org and A aq , respectively), meaning aqueous media 99% of water content in the sample (ESI Fig. S62 †).The synthetized family of compounds shows consistent absorption maxima, centered at ca. 280 and 360 nm (Fig. 1b) with minor changes between organic and aqueous solvent.However, 12.Br shows a minor shi in aqueous media, that becomes more evident with the increase in concentration (Fig. 1b).Further analysis of the A 360 dependence with the concentration (see S62 †) shows linearity, in good agreement with the Lambert-Beer law, for the whole series.
Subsequently, the emission spectra upon excitation at 360 nm is recorded in organic and aqueous media (I org and I aq , respectively).The photoluminescence intensity is shown at different concentrations for 12.Br in Fig. 1c and S62 † for the rest of the series.The general trend shows enhanced emission in aqueous media (I aq > I org ), which is in agreement with the AIE effect.In order to determine the extent of this increase through the series, Fig. 1d shows the ratio between I aq and I org at different concentrations.4.I shows limited solubility in organic solvents, and therefore cannot be dissolved in a concentration higher than 2.5 mM, limiting the concentration to 25 mM.
Furthermore, we consider a minimum threshold of threefold increase (marked as light green on the table) to be a relevant AIE effect.This threshold is a desirable noise-to-signal ratio in e.g., microscopy.The table at Fig. 1d highlights the interplay between the alkyl side chains and the electrostatic repulsions: only 12.Br above 12 mM shows an emission increase of 5.8, whereas 6.Br at the same concentration only displays an increase of 1.8 times.This exemplies the role of alkyl chains in the formation of emitting aggregates.Therefore, the optimized conditions of the series are obtained for [12.Br] = 50 mM, and thus, a thorough study at different water percentages was carried out at this concentration under these conditions.
First, the emitting properties at decreasing organic fraction solvents are recorded.The AIE effect as described above is turned on when the sample contains over 80% of water content (Fig. 1e).Notwithstanding, once aggregates are formed, the emission obtained for the sample at 99% of water is almost 13 times higher compared to in organic solvent (Fig. 1f).The relationship between aggregation and emitting properties is further conrmed by monitoring the size distribution measured by DLS at different water fractions.It was observed that aggregates start forming at 80% of water content in the sample (see ESI Fig. S66 †).Aer, structures reduce the diameter from 185 nm (80% water, DI: 0.178) to 115 nm (99% water, DI: 0.108).

Counterion chemistry as aggregation inducing emission parameter
Synthesis of the PF 6 TPPE-alkyl salts.Although the selected family of positively-charged AIEs has been achieved by side-chain chemistry, the desired AIE effect is only achieved upon conjugation with long (C 12 ) chains.Therefore, to further promote the hydrophobicity, the counterion exchange for more hydrophobic derivatives was explored.Hexauorophosphate anion (PF 6
Photophysical properties of the PF 6 TPPE-alkyl salts in solution.The PF 6 -family exhibits an updated hydrophilicity/ hydrophobicity balance, adding the counterion chemistry to the balance between the positively charged pyridinium moieties and the side chain length.This hinders the electrostatic repulsion more efficiently than solely sidechain chemistry and Fig. 2 (a) Synthetic path for ion exchange of the series.Scheme of the effect of the counterion modification in supramolecular driving forces that lead to monomeric or aggregated state in aqueous media.(b) UV-vis absorbance spectra of 6.PF 6 at different concentrations (full and dashed lines for sample in aqueous and organic media, respectively).(c) Ratio A org /A aq at 360 nm at different concentrations for 2.PF 6 , 4.PF 6 and 6.PF 6 , showing a sharp increase due to aggregation for 6.PF 6 .(d) A 360 at different concentrations for 6.Br in organic solvent (blue rhombus), 6.Br in aqueous media (green triangles), 6.PF 6 in organic solvent (yellow squares) and 6.PF 6 in aqueous media (red circles).The trendlines are marked with the same colour.In the case of 6. promotes self-aggregation in aqueous media (Fig. 2a).The absorbance spectra of PF 6 TPPE-alkyl salts are recorded at different concentrations for both, organic and aqueous media (Fig. S64 †).The PF 6 -family shows absorption maxima consistent with the halide derivatives, centred at ca. 280 and 360 nm (Fig. 2b).However, A aq displays a remarkable decrease compared to A org that becomes more evident with the increase in the concentration and the length of the alkyl chain and exemplied by 6.PF 6 (Fig. 2c and S64 †).The ratio between A org / A aq at 360 nm shows a sharp increase above 25 mM, as consequence of the heavy aggregation in aqueous media, and is accentuated with the increasing side-chain length.The counterion effect is more evident when comparing the halide counterpart.Plotting the A aq, at 360 nm for 6.Br and 6.PF 6 in both organic and aqueous media (Fig. 2d) shows an acute deviation of 6.PF 6 from the Lambert-Beer law (Fig. 2d, red circles) when concentration reaches 25 mM, a clear indication of saturation of the system, loss of colloidal stability, and eventual precipitation.In addition, the emission spectra upon excitation at 360 nm is recorded for the PF 6 -family in organic and aqueous media (see Fig. S64 †).The emission intensity of 6.PF 6 at different concentrations is shown in Fig. 2e and S64, † exhibiting a major emission enhancement in aqueous media when compared with the one in organic solvent.This is in line with the aggregation shown in the absorbance.To normalize the emission across the concentrations, the ratio between I aq and I org at given conditions is plotted again in a table (Fig. 2f).The table summarizes the subtle interplay that alkyl side chains, counterion, concentration, and electrostatic repulsions play in this system.The PF 6 -family shows an AIE effect with shorter side chains and lower concentrations (Fig. 2f vs. 1d).Moreover, the hydrophobicity introduced by C 12 chains in combination with a concentration increase is critical: [12.PF 6 ] = 5 mM exhibits an emission increment of 27.8, whereas [12.PF 6 ] = 12 mM is reduced to 19.4.A plausible explanation is the oversaturation of the system that leads to visible occulation and particle precipitation, hindering the accurate measurement in solution.This effect is observed with higher concentrations, thus reaching the limit of colloidal stability, and leading to quantitative precipitation.This poor colloidal behaviour limits the scope of further studies, and 12.PF 6 is not further studied.Fig. 2g shows the difference in emission between organic solvent and aqueous media, and the effect of the side chain length at 100 mM for the series.A more detailed understanding of the optimized conditions of the series (i.e.[6.PF 6 ] = 100 mM) is obtained by stepwise increase of the water content (Fig. 2h).First, the absorbance spectrum and the emitting properties are recorded under these conditions (Fig. 2h).The heavy decrease in A 360 at 80% of water, consistent with the increase of emission at 550 nm marks the conditions for aggregate formation.The size of this aggregates is further studied by DLS measurements (Fig. S66 †).At [6.PF 6 ] = 100 mM the autocorrelation is not suitable for tting, most likely due to i.e. precipitation.Therefore, further studies were carried out at 12 and 50 mM (Fig. 2i).Under these conditions, aggregates at 99% of water content in the sample shows sizes of 149.8 and 210.1 nm, respectively, although higher dispersities.This points towards a lower colloidal stability in water of the PF 6 -family, when compared with their halide counterparts.
Electrochemical characterization of the PF 6 TPPE-alkyl salts in solution.Altogether, the PF 6 family going from 1.PF 6 to 6.PF 6 derivatives show superior AIE properties, promising for their use in lighting devices. 31,32Thus, we turned to investigate the effect of the substitution pattern on the electrochemical behaviour using square wave voltammetry (SWV) in MeCN (Table 1 and Fig. S67 †).Though two well-dened sequential reductions at 1.36 V and 1.60 V are noted for all compounds, 1.PF 6 and 2.PF 6 showed a partial reversibility, while 4.PF 6 and 6.PF 6 are almost quasi reversible.This goes in line with the anodic process, in which multiple oxidation waves in the range of 1.0-2.5 V turned to be more dened and reversible with the increase of the alkyl chain length.Thus, it is expected that charge injection and transport will be critical for the device performance, while the increase of the alkyl chain provides the most promising redox behaviour (4.PF 6 and 6.PF 6 ) for the implementation into LECsvide infra.
Photophysical studies of the PF 6 TPPE-alkyl salts in thin lms.Thin lms (∼70-90 nm) were prepared on quartz via spincoating using MeCN solutions (see the Experimental section for details) following a vacuum (3 mbar for 50 min) drying process and a subsequent standard temperature treatment at 90 °C for 30 min under inert atmosphere, since the working temperature of LECs spans from 35-75 °C depending on the driving conditions. 34,35Atomic force microscopy (AFM) images (Fig. 3a and S69 †) of the thin lms conrmed a homogeneous morphology with neither apparent phase separation nor large aggregates and small hillocks formations related to the slow evaporation of MeCN upon lm forming.Overall, the root mean square (RMS) roughness value for all the lms was around 300 pm.The photoluminescence features (Fig. 3b and c) show broad emission band centred at 562 and 565 nm for 1.PF 6 and 2.PF 6 , further blue-shied to 555 nm and 552 nm for 4.PF 6 and 6.PF 6 , suggesting a different type of aggregation and/or molecular conformation induced by the length of the alkyl chain as expected from the solution studies.This is nicely reected in the photoluminescence quantum yields (PLQYs) that evolve from 68% and 67% (1.PF 6 and 2.PF 6 ) to 60% and 50% (4.PF 6 and 6.PF 6 ), while the excited state device lifetime values (s) are around 4 ns, as expected for a uorescence emission process.Thus, the benets of the AIE 4.PF 6 and 6.PF 6 also stand out in terms of thin-lm photoluminescence behaviour for LEC application.
Light-emitting electrochemical cells (LEC) with ionic AIE emitters.LECs were fabricated with a double-layered architecture ITO/PEDOT:PSS (70 nm)/active layer (∼70 nm)/Al (100 nm) and analysed by (i) static electrochemical impedance spectroscopy (EIS) to determine ion mobility features in the active layer, and (ii) monitoring the luminance, colour (x/y CIE colour coordinates), and electrical behaviour over time at pulsed current density of 100 mA cm −2 .7][38][39][40] In short, we applied a DC voltage at 0 V to an AC signal of 10 mV amplitude and at frequencies from 10 6 to 10 Hz.The Nyquist plots were analysed using a single resistor/ capacitor equivalent circuit (Fig. S70 †).A direct comparison between 1.PF 6 and 2.PF 6 (low AIE feature) and 4.PF 6 and 6.PF 6 (strong AIE feature) lms, shows that the lock-structure of AIE emitters slightly impact the 3 values that hold at ca. 8 (Fig. 3c).Likewise, all the devices showed a similar s value in the regime of 5-9 × 10 −7 S m −1 .Thus, 6.PF 6 systems can also build up EDLs and assist the growth of the electrochemical doped regions, regardless of the alkyl chains length compared to 1.PF 6 .Overall, these ndings are in line with the recent contribution of Edman, 23 corroborating that the lock morphology of AIE emitters allows ion polarization regardless of their neutral or ionic nature.
Next, we studied the electroluminescent behaviour of the LECs at pulsed current density of 100 mA cm −2 .As expected, all the devices exhibited a reduction of the applied voltage along with an increase of luminance response (Fig. 3e, f and S70 †).Indeed, an instantaneous brightness response associated to a broad emission spectrum centred at 550 nm and 560 nm for 1.PF 6 /2.PF 6 and 4.PF 6 /6.PF 6 , respectively.Thus, photo-/ electroluminescence band shapes and the maximum emission wavelength remains without notable variation for each molecule, indicating that the same excited state is involved regardless of the photo/electrical excitation process over time.(E 0- 0 and l max in Fig. 3c (PL) and Fig. 3i (EL).While the emission band is stable for 4.PF 6 /6.PF 6 devices, those of 1.PF 6 /2.PF 6 slightly red-shis over time due to the increase of the device temperature to ca. 45 °Cvide supra.Overall, the device chromaticity corresponds to a greenish emission as corroborated by the x/y CIE colour coordinates of 0.40-4/0.51-4.More interesting, the luminous efficiency and device brightness gradually increases with the length of the alkyl chain, reaching values of 0.07, 0.12, 0.16, and 0.19 lm W −1 and 13.38, 23.84, 36.20, and 49.54 cd m −2 for 1.PF 6 , 2.PF 6 , 4.PF 6 and 6.PF 6 devices (Fig. 3e  and f).This is nicely reected in the device stability studied using the total emitted energy (E tot ) that is calculated by integrating the radiant ux curve until the time needed to reach one-h of the maximum luminance as an upper limit denition (Fig. 3i). 22Here, E tot gradually increases from 0.47 mJ to 6.75 mJ upon increasing the alkyl length chain (Fig. 3i).Indeed, Fig. 3j displays a clear enhancement of the device efficiency and stability with the increase of the alkyl chain as expected by the higher and stable thin-lm PLQY under working conditionsvide supra.
However, a high PLQY does not directly imply the best performing device, since charge trapping and/or electrochemical doping critically alter the preferred composition of the active material. 41In this context, the enhanced reversibility of the electrochemical processes keeping a good ion polarizability in thin lms upon increasing the alkyl chain is also key towards circumventing hole injection/transport limitations.
To further conrm the benets of the AIE behaviour, we prepared another set of devices using an inert polymer matrix to disrupt aggregation, that is, adding 20 wt%. of polymethylmethacrylate (PMMA) with respect to the best emitting molecule 6.PF 6 (see Experimental section for details). 42As showed in Fig. 3k, the device performance with PMMA decreases considerably with a luminance from 49.54 (pristine) to 3.77 (with PMMA) cd m −2 , and an efficiency from 0.19 (pristine) to 0.022 (with PMMA) lm W −1 , corroborating that the aggregation induced emission is, indeed, crucial for this type of emitters.

Conclusions
In summary, two different families of positively charged structures derived from TPPE were successfully synthetized, and the one with optimized performance applied in ion-based lighting devices, such as LECs, to rationalize the effect of the hydrophobic/hydrophilic forces (represented by the positively charged pyridinium moieties and the increasing chain length and counterion, respectively) that govern the AIE behaviour.For instance, halide AIE series require C 12 side chain lengths to overcome the inherent electrostatic repulsions and selfaggregation, while PF 6 − AIE series increases the hydrophobic nature promoting the aggregate formation and gradually enhancing their emitting properties from C2 up to C6 side chains.This was nicely corroborated by the gradual PLQY increase going from 1.PF 6 to 6.PF 6 lms.In addition, a reasonable electrochemical behaviour that allows their integration in LECs was also noted in the PF 6 − series.Here, the devices featured a gradually enhanced brightness, efficiency and stability going from 1.PF 6 to 6.PF 6 emitters, indicating that the AIE feature is benecial.Indeed, EIS assays corroborated that the lock structure of AIE emitters allows and efficient ion polarization regardless of their neutral or ionic nature; 23 a question that has always discouraged the community to apply this type of materials in LECs.Finally, we also state that the AIE feature is key towards meeting high performance by using PMMA additive that disrupt the formation of aggregates LECs and, in turn, dramatically reduced the device performance of 6.PF 6 AIE emitter.Overall, this work rationalizes a design guideline for ionic AIE emitters with ne-tuned colloidal stability, encouraging their future application in water-based applications such nanomedicine or sensor or, as in this case, light-management technologies like lighting emitting electrochemical cells.

Fig. 1
Fig. 1 (a) Schematic representation of the TPE derivatives, as well as the key design features and supramolecular driving forces leading to monomeric or aggregating state in aqueous media.(b) UV-vis absorbance spectra of 12.Br at different concentrations (full and dashed lines for sample in aqueous and organic media, respectively).(c) Emission spectra of 12.Br at different concentrations (full and dashed lines for sample in aqueous and organic media, respectively) upon excitation at 360 nm.(d) Ratio I aq /I org at maximum of emission (550 nm) at varying concentrations of the series.In light green and green are marked results with a ratio of 3 and 3.1-30, respectively.(e) Image of 12.Br ([12.Br] = 50 mM) titration at different water fraction content, showing increased emission above 80% of water.(f) Titration of [12.Br] = 50 mM at varying water percentage.Absorbance (orange line) at 360 nm and emission (green line) at 550 nm upon excitation at 360 nm.A sharp increase can be found above 80% water/MeOH mixture.(g) Volume-averaged particle size distribution of [12.Br] = 50 mM measured by DLS, showing high dispersity at 80% and size stabilization at 90% and above.No data was obtained for solutions below 80% water, indicating lack of aggregates.Inset: second order normalized autocorrelation function of the selected samples.Dispersity index (DI) and volume-averaged hydrodynamic diameter (D h av.) correspond to average obtained after three repetitions of 12.Br at 99% water/MeOH mixture.
Fig.2(a) Synthetic path for ion exchange of the series.Scheme of the effect of the counterion modification in supramolecular driving forces that lead to monomeric or aggregated state in aqueous media.(b) UV-vis absorbance spectra of 6.PF 6 at different concentrations (full and dashed lines for sample in aqueous and organic media, respectively).(c) Ratio A org /A aq at 360 nm at different concentrations for 2.PF 6 , 4.PF 6 and 6.PF 6 , showing a sharp increase due to aggregation for 6.PF 6 .(d) A 360 at different concentrations for 6.Br in organic solvent (blue rhombus), 6.Br in aqueous media (green triangles), 6.PF 6 in organic solvent (yellow squares) and 6.PF 6 in aqueous media (red circles).The trendlines are marked with the same colour.In the case of 6.PF 6 , there is a trendline based on the three first concentrations and a second trendline (light red) corresponding to the results at 25, 50 and 100 mM highlighting the self-aggregation at these concentrations.(e) Emission spectra of 6.PF 6 at different concentrations (full and dashed lines for samples in aqueous and organic media, respectively) upon excitation at 360 nm.(f) Ratio I aq /I org at maximum of emission (550 nm) at varying concentrations of the PF 6 -family compounds.Different green intensities have been used to emphasize the AIE effect.At [12.PF 6 ] > 12 mM sample not soluble in water.(g) Images of 1.PF 6 , 2.PF 6 , 4.PF 6 and 6.PF 6 (left to right) at 100 mM in organic solvent (upper row) and aqueous media (lower row).(h) Titration of [6.PF 6 ] = 50 mM varying water percentage.Absorbance results at 360 nm and fluorescence results at 550 nm by excitation at 360 nm.(i) Volume-averaged particle size distribution of [6.PF 6 ] = 12 mM (yellow) and 50 mM (green) in aqueous media measured by DLS.Inset: second order normalized autocorrelation function of the selected samples.DI and D h av.correspond to average obtained after three repetitions at 99% water/MeOH mixture.

Fig. 3
Fig. 3 (a) AFM topography of the 6.PF 6 film dried under vacuum treatment, and its profile (bottom).(b) Excitation and emission spectra (dashed and full lines, respectively) in thin films.(c) Photoluminescence features of the films.(d) Pictures under UV illumination (305 nm) of the thin films deposited on quartz.(e) Luminance and (f) efficiency of the LECs.(g) Normalized electroluminescence spectra of the devices.(h) Schematic of the device's architecture, in addition to an optical image of a device's pixel in operando.(i) Devices performance at pulsed current density driving of 100 mA cm −2 .LECs prepared with 6.PF 6 mixed with PMMA (6.PF 6 -PMMA) to disrupt aggregation.(j) Efficiency (yellow) and total emitted energy (red) in relationship with alkyl chains length.(k) Luminance (red) and efficiency (yellow) of LECs made with 6.PF 6 -PMMA.

Table 1
Electrochemical features vs. Fc/Fc + of 1.PF 6 , 2.PF 6 , 4.PF 6 and 6.PF 6 in MeCN/NBu 4 PF 6 (0.1 M) Finland Centers of Excellence Program (2022-2029) in Life-Inspired Hybrid Materials (LIBER) 346110.OA-R and RDC thanks the funding from the European Union's Horizon 2020 research and innovation program under the Marie Skłodowska-Curie grant agreement No. 899987.LMC and RDC acknowledged the European Union's MSCA-ITN programme under grant agreement STiBNite No. 956923.We are also thankful to the Aalto Internal Funding Call 2022 -For Cooperation Initiatives with Technical University of Munich (TUM).We acknowledge the provision of facilities and technical support by Aalto University Bioeconomy and Raw Materials Research Infrastructure (RAMI) facilities.